CHAPTER

1

Background on

Mechanics of Materials

CHAP TE R

1.1

Background on

Modeling

J

EAN

L

EMAITRE

Universit

!

e Paris 6 }LMT Cachan,61 av.du pr

!

esident Wilson,F-94235 Cachan Cedex,France

Contents

1.1.1 Introduction..................................3

1.1.2 Observations and Choice of Variables.........4

1.1.2.1 Scale of observation...................5

1.1.2.2 Internal Variables......................6

1.1.3 Formulation..................................6

1.1.3.1 State Potential.........................7

1.1.3.2 Dissipative Potential...................8

1.1.4 Identiﬁcation.................................9

1.1.4.1 Qualitative Identiﬁcation...............9

1.1.4.2 Quantitative Identiﬁcation............11

1.1.5 Validity Domain.............................13

1.1.6 Choice of Models............................13

1.1.7 Numerical Implementation...................14

Bibliography.......................................14

1.1.1 INTRODUCTION

Modeling,as has already been said for mechanics,may be considered ‘‘a

science,a technique,and an art.’’

It is science because it is the process by which observations can be put

in a logical mathematical framework in order to reproduce or simulate

related phenomena.In mechanics of materials constitutive equations relate

loadings as stresses,temperature,etc.to effects as strains,damage,fracture,

wear,etc.

Handbook of Materials Behavior Models

Copyright#2001 by Academic Press.All rights of reproduction in any form reserved.

3

It is a technique because it uses tools such as mathematics,thermo-

dynamics,computers,and experiments to build close form models and to

obtain numerical values for the parameters that are used in structure

calculations to predict the behavior of structures in the service or forming

process,etc.,safety and optimal design being the main motivations.

It is an art because the sensibility of the scientist plays an important role.

Except for linear phenomena,there is not unique way to build a model froma

set of observations and test results.Furthermore,the mathematical structure

of the model may depend upon its use.This is interesting from the human

point of view.But it is sometimes difﬁcult to select the proper model for a

given application.The simplest is often the more efﬁcient event,even if it is

not the most accurate.

1.1.2 OBSERVATIONS AND CHOICE

OF VARIABLES

First of all,in mechanics of materials,a model does not exist for itself;it exists

in connection with a purpose.If it is the macroscopic behavior of mechanical

components of structures that is being considered,the basic tool is the

mechanics of continuous media,which deals with the following:

1.Strain,a second-order tensor related to the displacement

~

u of two points:

Euler’s tensor

e for small perturbations.

e

ij

¼

1

2

ðu

i;j

þu

j;i

Þ

ð1Þ

In practice,the hypothesis of ‘‘small’’ strain may be applied if it is below

about 10%.

Green-Lagrange tensor

D (among others) for large perturbations,if F is

the tangent linear transformation which transforms under deformation a

point M

0

of the initial conﬁguration into M of the actual conﬁguration.

d

~

xðMÞ ¼

%

Fd

~

XðM

0

Þ

D ¼

1

2

ð

%

F

T

%

F

%

1Þ

ð2Þ

With

F

T

the transpose of

%

F.

2.Stress,a second-order tensor dual of the strain tensor;its contracted

product by the strain rate tensor is the power involved in the mechanical

process.

Lemaitre

4

Cauchy stress tensor s for small perturbations,checking the equilibrium

with the internal forces density

~

f and the inertia forces r

.

~

u;

s

ij;j

þf

i

¼ r

.

u

i

with

.

u

i

¼

d

2

u

dt

2

ð3Þ

Piola-Kirchoff tensor

%

S (among others) for large perturbations.

%

S ¼ detð

%

FÞ

s

%

F

T

ð4Þ

3.Temperature T.

These three variables are functions of the time t.

1.1.2.1 S

CALE OF

O

BSERVATION

From the mathematical point of view,strains and stresses are deﬁned on a

material point,but the real materials are not continuous.Physically,strain

and stress represent averages on a ﬁctitious volume element called the

representative volume element (RVE) or mesoscale.To give a subjective order

of magnitude of a characteristic length,it can be

0.1mm for metallic materials;

1mm for polymers;

10mm for woods;

100mm for concrete.

It is below these scales that observations must be done to detect the

micromechanisms involved in modeling:

– slips in crystals for plasticity of metals;

– decohesions of sand particles by breaking of atomic bonds of cement for

damage in concrete;

– rupture of microparticles in wear;

– etc.

These are observations at a microscale.It is more or less an ‘‘art’’ to decide at

which microscale the main mechanism responsible for a mesoscopic

phenomenon occurs.For example,theories of plasticity have been developed

at a mesoscale by phenomenological considerations,at a microscale when

dealing with irreversible slips,and now at an atomic scale when modeling the

movements of dislocations.

At any rate,one’s ﬁrst priority is to observe phenomena and to select the

representative mechanism which can be put into a mathematical framework

1.1 Background on Modeling

5

of homogenization to give variables at a mesoscale compatible with the

mechanics of continuous media.

1.1.2.2 I

NTERNAL

V

ARIABLES

When the purpose is structural calculations with sets of constitutive

equations,it is logical to consider that each main mechanism should have

its own variable.For example,the total strain

e is directly observable and

deﬁnes the external state of the representative volume element (RVE),but for

a better deﬁnition of the internal state of the RVE it is convenient to look at

what happens during loading and unloading of the RVE to deﬁne an elastic

strain

e

e

and a plastic strain

e

p

such as

e

ij

¼ e

e

ij

þe

p

ij

ð5Þ

The elastic strain represents the reversible movements of atoms,and the

plastic strain corresponds to an average of irreversible slips.

All variables which deﬁne the internal state of the RVE are called internal

variables.They should result from observations at a microscale and from a

homogenization process:

– isotropic hardening in metals related to the density of dislocations;

– kinematic hardening related to the internal residual microstresses at the

level of crystals;

– damage related to the density of defects;

– etc.

How many do we need?As many as the number of phenomena taken into

consideration,but the smallest is the best.

Finally,the local state method postulates that the considered thermo-

dynamic state is completely deﬁned by the actual values of the corresponding

state variables:observable and internal.

1.1.3 FORMULATION

The thermodynamics of irreversible processes is a general framework that is

easy to use to formulate constitutive equations.It is a logical guide for

incorporating observations and experimental results and a set of rules for

avoiding incompatibilities.

The ﬁrst principle is the energy balance:If e is the speciﬁc internal energy,

r the density,o the volume density of internal heat produced by external

Lemaitre

6

sources,and

~

q The heat ﬂux:

r

’

e ¼ s

ij

’

e

ij

þoq

i;i

ð6Þ

The second principle states that the entropy production

’

s must be larger or

equal to the heat received divided by the temperature

r

’

s

o

T

q

i

T

;i

ð7Þ

If c ¼ e Ts is the Helmholtz speciﬁc free energy (this is the energy in the

RVE which can eventually be recovered),

s

ij

’

e

ij

rð

’

cþs

’

TÞ

q

i

T

;i

T

0

ð8Þ

This is the Clausins-Duhem inequality,which corresponds to the positiveness

of the dissipated energy and which has to be fulﬁlled by any model for all

possible evolutions.

1.1.3.1 S

TATE

P

OTENTIAL

The state potential allows for the derivation of the state laws and the

deﬁnition of the associate variables or driving forces associated with the state

variables V

K

to deﬁne the energy involved in each phenomenon.Choosing the

Helmholtz free energy c,it is a function of all state variables concave with

respect to the temperature and convex with respect to all other V

K

,

c ¼ cð

e;T;e

e

;

e

p

;...V

K

...Þ ð9Þ

or in classical elastoplasticity

c ¼ cð

e

e

;

e

p

;T;...V

K

...Þ ð10Þ

The state laws derive fromthis potential to ensure that the second principle is

always fulﬁlled.

s

ij

’

e

p

ij

X

r

@c

@V

K

’

V

K

q

i

T

;i

T

0

ð11Þ

They are the laws of thermoelasticity

s

ij

¼ r

@c

@e

e

ij

ð12Þ

s ¼

@c

@T

ð13Þ

1.1 Background on Modeling

7

The associated variables are deﬁned by

s

ij

¼ r

@c

@e

p

ij

ð14Þ

A

K

¼ r

@c

@V

K

ð15Þ

Each variable A

K

is the main cause of variation of the state variable V

K

.In

other words,the constitutive equations of the phenomenon represented by

V

K

will be primarily a function of its associated variable and eventually

from others.

’

V

K

¼ gð...A

K

...Þ ð16Þ

They also allow us to take as the state potential the Gibbs energy dual of the

Helmholtz energy by the Legendre-Fenchel transform

c

*

¼ c

*

ð

s;s;...A

K

...Þ ð17Þ

or any combination of state and associated variables by partial transform.

1.1.3.2 D

ISSIPATIVE

P

OTENTIAL

To deﬁne the g function of the kinetic equations,a second potential is

postulated.It is a function of the associate variables,and convex to ensure

that the second principle is fulﬁlled.It can also be a function of the state

variables but taken only as parameters.

j ¼ jð

s;...A

K

...;grad

!

T;

e

e

;T;...V

K

...Þ

ð18Þ

The kinetic laws of evolution of the internal state variables derive from

’

e

p

ij

¼

@j

@s

ij

ð19Þ

’

V

K

¼

@j

@A

K

ð20Þ

~

q

T

¼

@j

@grad

!

T

ð21Þ

Unfortunately,for phenomena which do not depend explicitly upon the time,

this function is not differentiable.The ﬂux variables are deﬁned by the

subdifferential of j.If F is the criterion function whose the convex F¼0 is the

Lemaitre

8

indicatrice function of j.

j ¼ 0 if F50!

’

e

p

¼ 0

j ¼ 1 if F ¼ 0!

’

e

p

6¼ 0

(

ð22Þ

Then,some mathematics prove that

’

e

p

ij

¼

@F

@s

ij

’

l

’

V

K

¼

@F

@A

K

’

l

if F ¼ 0 and

’

F ¼ 0 ð23Þ

’

e

p

ij

¼ 0

’

V

K

¼ 0

if F50 or

’

F50 ð24Þ

This is the generalized normality rule of standard materials for which

’

l is the

multiplier calculated by the consistancy condition f ¼ 0;

’

f ¼ 0.

1.1.4 IDENTIFICATION

The set of constitutive equations is fully deﬁned if the two potentials c and f

take appropriate close forms:this is the qualitative identiﬁcation.The numerical

response of the constitutive equations to any input is obtained if the materials

parameters take the appropriate values:this is the quantitative identiﬁcation.

1.1.4.1 Q

UALITATIVE

I

DENTIFICATION

Assume an interest in several phenomena for which q internal variables have

been identiﬁed.Which functions should one choose for cð

e

e

;

e

p

;T;V

1

...V

q

Þ

and jð

s;A

1

...A

q

;grad

!

T;

e

e

;T;V

1

...V

q

Þ?

If a phenomenon is known as linear,the corresponding potentials are

positive deﬁnite quadratic functions.For linear elasticity,for example,

c

e

¼

1

2r

E

ijkl

e

e

ij

e

e

kl

ð25Þ

where r is the density and

E the Hooke tensor.

If two phenomena I and J are known to be coupled,the corresponding

potentials should verify

a state coupling:@

2

c=@V

I

@V

J

6

¼ 0

or an evolution coupling:@

2

j=@V

I

@V

J

6

¼ 0

If no coupling occurs @

2

c=@V

I

@V

J

¼ 0 and @

2

j=@V

I

@V

J

¼ 0.

1.1 Background on Modeling

9

Following is an example of elasticity coupled to damage represented by the

variable D:

@

2

c

@D@e

e

ij

6¼ 0

ð26Þ

c

e

¼

1

2r

E

ijkl

e

e

ij

e

e

kl

H

1

ðDÞ multiplication of functions

ð27Þ

s

ij

¼ r

@c

e

@e

e

ij

¼ E

ijkl

e

e

ij

H

1

ðDÞ

ð28Þ

If such coupling would not have existed,we would have written

c

e

¼

1

2r

E

ijkl

e

e

ij

e

e

kl

þH

2

ðDÞ addition of functions

ð29Þ

that is,@

2

c=@D@e

e

ij

¼ 0

s

ij

¼ r

@c

e

@e

e

ij

¼ E

ijkl

e

e

ij

ð30Þ

For nonlinear phenomena,often power functions are used,but for

phenomena which asymptotically saturate,exponential functions are

preferred.Often this choice is subjective.Nevertheless,micromechanics

analysis may yield logical functions with regard to the micromechanisms

introduced at microscale.It consists of the calculation of the energy involved

in a RVE by a proper integration or an average of the elementary energies

corresponding to the micromechanisms considered.

Qualitative experiments are used to point out the tendencies of evolution,

but they do not concern the potentials in themselves because simple direct

measurements of energy is not possible.Measurements concern the evolution

of variables:strain as a function of stress,crack length as a function of time,

etc.This means that the potentials are identiﬁed froman integration of what is

observed.For example,an observation of the secondary creep plastic strain

rate as a nonlinear function of the applied stress in creep tests given by the

phenomenological Norton law

’

e

p

¼ ðs=KÞ

N

is introduced in the dissipative

potential as

j ¼

K

Nþ1

s

eq

K

Nþ1

ð31Þ

if some multiaxial experiments show that the von Mises criterion is fulﬁlled

(s

eq

is the von Mises equivalent stress).

Lemaitre

10

1.1.4.2 Q

UANTITATIVE

I

DENTIFICATION

This is the weakest point of the mechanics of materials.All the parameters

introduced in constitutive equations (Young’s modulus E and Poisson’s ratio n

in elasticity,Norton’s parameters K and N in creep,etc.) differ for each

material and are functions of the temperature.Since there are thousands of

different materials used in engineering and since they change with the

technological progress of elaboration processes,there is no way to built

deﬁnite,precise databases.Another point is that when a structural calculation

is performed during a design,the deﬁnitive choice of materials is not

achieved,and,even if it is,nobody knows what the precise properties of the

materials elaborated some years after will be.The only solution is to perform

the structural calculations with the models identiﬁed with all known

information and to update the calculations each time a new piece of

information appears,even during the service of the structure.This,of course,

necessitates close cooperation between the designers and the users.

1.1.4.2.1 Sensibility to Parameters

When a model is being used,all material parameters do not have the same

importance for the results:a small variation of some of them may change the

results by a large amount,whereas a large variation of others has a small

inﬂuence.For example,a numerical sensibility analysis on the parameters s

y

,

K,and Mon the shape of the stress-strain curve,graph of the simple model of

uniaxial plasticity

s ¼ s

y

þKe

1=M

p

ð32Þ

shows that the more sensible parameter is s

y

;by taking an approximate value

of M (M¼3,4,5),it is always possible to adjust K in order to have a

satisfactory agreement.But a good correlation with the set of available data

does not prove that the model is able to give satisfactory results for cases far

away from the tests used for the identiﬁcation.

Before any quantitative identiﬁcation of a model is made,it is advisable to

perform a sensibility analysis in order to classify by increasing order of

sensibility the parameters s

y

,K,and M and to proceed as follows:

1.1.4.2.2 Rough Estimation of Parameters

From all known data,make a ﬁrst estimation of the parameters using all

approximations in the model in order to have the same number of unknowns

as the number of pieces of information.Eventually,take values of parameters

corresponding to materials that are close in their chemical composition.

1.1 Background on Modeling

11

Continue with the same example of the preceding plasticity model for a

mild steel for which s

y

is known as 300MPa.If the ultimate stress s

u

is known

as 400 MPa for a plastic strain to rupture e

pu

0.20,then taking M¼1 allows

one to ﬁnd K500MPa.

These approximate values of the parameters may be taken as a starting

solution of an optimization process.

1.1.4.2.3 Optimization Procedure

If now more experimental results are available,an optimization procedure

may be performed to minimize the difference between the test data and the

prediction of those tests by the full numerical resolution of the model.The

least-square method is advantageously used.

Unfortunately,in the range of nonlinear models,the minimization of the

error function may have several solutions due to local minima or ﬂat

variations for which the gradient methods converge extremely slowly.This is

why the starting solution should be as close as possible to the optimized

solution and why one should give different weight factors to the parameters

in order ‘‘to help’’ the numerical procedure:small weight factors to less

sensible parameters.

1.1.4.2.4 Validation

The process is not ﬁnished until the model has been applied and compared to

special tests which have not been used for the identiﬁcation.Of course,the

model should be applied to the identiﬁcation cases,but this is only for

checking the identiﬁcation procedure.

These validation tests must be as close as possible to the case considered

for applications,and as far as possible fromthe identiﬁcation tests }close or

far in the sense of variables.For example:

– biaxial tests if the tests of identiﬁcation were uniaxial;

– nonisothermal tests if the tests of identiﬁcation were conducted at

constant temperature;

– tests with gradient of stress or of other variables;

– different time scales;

– etc.

The comparison between validation tests and prediction gives concrete ideas

about the applicability of the models from the point of view of accuracy

and robustness.

Lemaitre

12

1.1.5 VALIDITY DOMAIN

Sometimes people say that ‘‘a good model should only be used to interpolate

between good tests.’’ I do not agree with this pessimistic view because to

interpolate between tests results a ‘‘good polynome’’ is sufﬁcient.A model is

something more.First,it includes ideas on the physical mechanisms involved;

second,it is a logical formulation based on general concepts;and third,only

after that,it is numbers.

The domain of validity of a model is the closed domain in the space of

variables inside which any resolution of the model gives an acceptable

accuracy.For the preceding model of plasticity,this is 05s5400MPa,

05e

p

50.2 for a relative accuracy of about de

p

=e

p

10% on plastic strain for

a given stress.

The bounds are difﬁcult to determine;they are those investigated by the

identiﬁcation tests program,plus ‘‘motivated’’ extrapolations based on well-

established concepts.Time extrapolation is the most crucial because the

identiﬁcation procedure deals within a time range of hours,days,or months,

whereas the applications of models deal within a time range of years or

decades.In such long periods of time phenomena of aging and changing

properties can occur which may be not included in the models.Aging

and change of properties by ‘‘in-service incidents’’ are certainly still

open problems.

1.1.6 CHOICE OF MODELS

The best model for a given application must be selected with much care and

critical analysis.First of all,investigate all the phenomena which may occur

and which have to be checked in the application:for example,monotonic or

cyclic plasticity.

Then determine the corresponding variables which should exist in the

model:for example,cyclic plasticity needs a kinematic hardening variable.

Check the domain of validity of the possible models in comparison to what

is expected in the application and select the simplest that has a good ratio of

quality to price,the quality being the accuracy and the price the number of

materials parameters to identify.

The choice of the model depends also on the available data to identify the

material parameters for the material concerned.Fortunately,often the

structural calculations are performed to compare different solutions in order

to optimize a design.In that case,good qualitative results are easily obtained

with rough estimations of the parameters.

1.1 Background on Modeling

13

1.1.7 NUMERICAL IMPLEMENTATION

The last activity in modeling is the numerical use of the models.Most of them,

in mechanics of materials,are nonlinear,incremental procedures and are used

together with iterations.For example,in plasticity:

– In a ﬁrst step the incremental strain ﬁeld is calculated by means of the

kinetic equations from momentum equations.

– The second step concerns the integration of the constitutive equations to

obtain the increments of the state variables and their new values.

– The third step consists in checking the momentum balance equation for

the actual stresses;if violated the iteration process goes to step 1 until a

given accuracy is obtained.

The Newton-Raphson method is often used.Implicit schemes in quasi-

static conditions or explicit schemes in dynamic conditions are used until the

end of the loading history or if a divergence appears as a loss of ellipticity or a

strain localization characteristic of softening behavior.

BIBLIOGRAPHY

Ashby,M.,and Jones,D.(1987).Engineering Materials,vols.1 and 2,Pergamon.

Fran

,

cois,D.,Pineau,A.,and Zaoui,A.(1998).Mechanical Behavior of Materials,vols.1 and 2,

Kluwer Academic Publishers.

Lemaitre,J.,and Chaboche,J.L.(1995).Mechanics of Solid Materials,Cambridge:Cambridge

University Press.

Lemaitre

14

CHAP TE R

1.2

Materials and Process

Selection Methods

Y

VES

B

RECHET

38402 St Martin d’Heres Cedex,France

Contents

1.2.1 Introduction.................................15

1.2.2 Databases:The Need for a Hierarchical

Approach....................................16

1.2.3 Comparing Materials:The Performance

Index Method...............................19

1.2.4 The Design Procedure:Screening,Ranking,

and Further Information,the Problem of

Multiple Criteria Optimization...............22

1.2.5 Materials Selection and Materials

Development:The Role of Modeling..........24

1.2.6 Process Selection:Structuring the Expertise..26

1.2.7 Conclusions.................................26

References.........................................28

1.2.1 INTRODUCTION

Designing efﬁciently for structural applications requires both a proper

dimensioning of the structure (involving as a basic tool ﬁnite element

calculations) and an appropriate choice of the materials and the process used

to give them the most suitable shape.The variety of materials available to the

engineer (about 80,000),as well as the complex set of requirements which

deﬁne the most appropriate material,lead to a multicriteria optimization

problem which is in no way a trivial one.In recent years,systematic methods

for materials and process selection have been developed [1–4] and

Handbook of Materials Behavior Models

Copyright#2001 by Academic Press.All rights of reproduction in any form reserved.

15

implemented into selection softwares [5–7] which ideally aim at selecting

the best materials early enough in the design procedure so that the best

design can be adequately chosen.This selection guide is most crucial

at the early stages of design:there would be no hope of efﬁciently

implementing a polymer matrix composite solution on a design initially

developed for a metallic solution.Selecting the most appropriate materials is a

task which should be done at the very beginning of the design procedure

and all along the various steps,from conceptual design to detail design

through embodiment design.The coupling with other design tools should at

the very least provide ﬁnite element codes with constitutive behavior

for the materials which appear the most promising.A more ambitious

program,yet to be implemented,is to interface these elements with expert

systems which would guide the designer toward shapes,processes more

suited to a given class of materials,and which ultimately would help

to redesign the component in an iterative manner according to the

materials selection.

These methods require databases of materials and tools to objectively

compare materials for a given set of requirements.The amount of modeling

needed in these methods is still quite elementary.In the present paper,we will

focus on the tools used to compare materials rather than on their

implementation as computer software.The modeling involved in the

performance index method (Section 1.2.2) is standard strength of materials.

The search for an optimal solution sometimes requires more reﬁned

optimization techniques (Section 1.2.3).We will outline in Section 1.2.4

the possible use of micromechanics and optimization methods in the

development of materials with the aim of meeting a giving set of

requirements.In Section 1.2.5 we will illustrate the need to structure and

store the expertise in process selection,and will outline the need for modeling

in this area.

1.2.2 DATABASES:THE NEED FOR A

HIERARCHICAL APPROACH

Material selection methods are facing a dilemma:the structure of the

databases and the selection tools have to be as general as possible to be easily

adaptable to a variety of situation.But this general structure is bound to fail

when the selection problem is very speciﬁc (such as,for instance,selecting

cast alloys).The methodology for materials selection presented in this paper

is a compromise in this dilemma.We will present ﬁrst the generic approach,

and then some speciﬁc applications.The idea is always to go from the

Brechet

16

most generic approach to the most speciﬁc one.In order to do so,the

materials databases have to be organized in a hierarchical manner so

that the selection at a given level orients the designer toward a more

speciﬁc tool.

Depending on the stages of design at which one considers the question of

materials selection,the level of information required will be different [1].In

the very early stages,all possible materials should be considered,and

therefore a database involving all the materials classes is needed.Accordingly,

at this level of generality,the properties will be stored as ranges with

relatively low precision.When the design procedure proceeds,more and more

detailed information is needed on a number of materials classes diminishing.

Properties more speciﬁc to,say,polymers (such as the water intake

or the ﬂammability) might be referred to in the set of requirements.In the last

stages of design,a very limited number of materials,and ﬁnally one

material and a provider,have to be selected:at this lever,very

precise properties suitable for dimensioning the structure are needed.

This progressive increase in specialization motivates a hierarchical approach

to databases used in materials selection tools:instead of storing all

the possible properties for a huge number of materials,which is bound to

lead to a database loaded with missing information,the choice has been to

develop a series of databases incorporating each a few hundreds of

materials.The generic database comprises metals,polymers,ceramics,

composites,and natural materials.Specialized databases have been developed

for steels,light alloys,polymers,composites,and woods.More specialized

databases coupling the materials and the processes (such as cast alloys,or

polymer matrix composites) can then be developed,but their format is

different from the previous databases.

The set of requirements for structural applications is very versatile.Of

course,mechanical properties are important (such as elastic moduli,yield

stresses,fracture stresses,or toughness).These properties can be stored as

numerical values.But very often,information such as the possibility of getting

the materials as plates or tubes,the possibility of painting or joining it

with other materials,or its resistance to the environment chemically

aggressive are as important.All the databases currently developed contain

numerical information,qualitative estimates,and boolean evaluations.More

recent tools [6] also allow one to store not only numbers,but also curves

(such as creep curves for polymers,at a given temperature under a given

strength).When a continuumset of data has to be stored,such as creep curves

or corrosion rates,being able to rely on a model with a limited number of

parameters (such as Norton’s law for creep) considerably increases the

efﬁciency of the storing procedure.For a database to be usable for selection

purposes,it should be complete (sometimes needing some estimation

1.2 Materials and Process Selection Methods

17

procedure),it should not overemphasize one material with respect to the

others,and it should contain data which are meaningful for all the materials

in the database.

The databases used in materials selection are of two types:either they list

the materials which are possible candidates,or they store the elements from

which the possible candidates are made.The ﬁrst case is rather simple;

provided a correct evaluation function is deﬁned,the ranking of the

candidates can be done by simple screening of the database.The second

case,for instance,when the database lists the resins and the ﬁbers involved in

making a composite material,requires both micromechanical tools to evaluate

the properties of the materials fromthe ones of its components,and also more

subtle numerical methods that are able to deal with a much larger (virtually

inﬁnite) set of possible candidates.Steepest gradient methods,simulated

annealing,and genetic algorithms are possible solutions for these complex

optimization problems.

In principle,one should try to select materials and processes simulta-

neously,since it is very often in terms of competition between various

couples (materials=processes) that the selection problem ﬁnally appears:

should one make an aiplane wing joining components obtained from

medium-thickness plates of aluminum alloys,or should one machine inside

a thick plate of a less quench sensitive alloy the wing together with the

stiffeners?The coupling between processes and materials properties is still

very poorly taken into account in the current selection procedures.Processes

are also selected from databases of attributes for the different processes

(such as the size of the components,the dimensional accuracy,or the

materials accessible to a given process).The databases for process

attributes have the same structure as the ones for materials,and the same

hierarchical organization,and information can be numeric,qualitative,

or boolean.

Beside the variety of properties (for materials) and attributes

(for processes) involved in a selection procedure,depending on the stage

of selection,one is either confronted with a very open end set of requirements,

or with always the same set of questions.In the ﬁrst situation,one

needs a very versatile tool,but because of combinatoric explosion,one cannot

afford to deal with questions involving interactions that are too complex

between various aspects,(such as ‘‘this shape,for this alloy,assuming

this minimal dimension,is prone during casting to exhibit hot tearing’’).

On the other hand,when the selection becomes very focused (such as

selection of joining methods),the set of requirements to be fulﬁlled has

basically always the same format:it can be stored as a ‘‘predeﬁned

questionnaire’’ which allows more reﬁned questions to be asked since they

are in a limited number.

Brechet

18

1.2.3 COMPARING MATERIALS:THE

PERFORMANCE INDEX METHOD

The databases are the hard core of the selection procedure:up to a certain

point they can be cast in a standard format,which has been used in CMS,CPS,

and CES software.When selection reaches a high degree of specialization,

more speciﬁc formats have to be implemented,and a questionnaire approach

rather than an ‘‘open-end selection’’ might be more efﬁcient.But a database

would be of little use without an evaluation tool able to compare the different

materials.Simple modeling allows one to build such a tool,but the price to be

paid is that dimensioning of the structure using this method is very crude.

One has to keep in mind that the aim is to identify the materials for which

accurate structural mechanics calculations will have to be performed later on.

Each set of requirements has to be structured in a systematic manner:What

are the constraints?What are the free and the imposed variables?What is the

objective?For instance,one might look for a tie for which the length L is

prescribed and the section S is free (free and imposed dimensions),which

shouldn’t yield under a prescribed load P (constraints),and which should be

of minimum weight (objective).The stress which should not exceed the yield

stress is

P

S

s

y

ð1Þ

The mass of the component to be minimized is

M ¼ r:L:S ð2Þ

The constraint not to yield imposes a minimum value for the section S.The

mass of the component is accordingly at least equal to

M

min

¼

r

s

y

L:Pð Þ

ð3Þ

Therefore,the material which will minimize the mass of the component will

be the one which maximizes the ‘‘performance index’’ I:

I ¼

s

y

r

ð4Þ

This very simple derivation illustrates the method for obtaining performance

indices:write the constraint and the objectives,eliminate the free variable,

and identify the combination of materials properties which measures the

efﬁciency of materials for a couple (constraints=objectives).These perfor-

mance indices have now been derived for many situations corresponding to

simple geometry (bars,plates,shells,beams) loading in simple modes

(tension,torsion,bending),for simple constraints (do not yield,prescribed

1.2 Materials and Process Selection Methods

19

stiffness,do not buckle...),and for various objectives (minimum weight,

minimum volume,minimum cost).They have been extended to thermal

applications.The way to derive a performance index for a real situation is to:

– simplify the geometry and the loading;

– identify the free variables;

– make explicit the constraint using simple mechanics;

– write down the objective;and

– eliminate the free variables between the constraint and the objectives.

TABLE 1.2.1 Classical performance indices for mechanical design for strength or stiffness at

minimum weight.

Objective Shape Loading Constraint

Performance

index

Stiffness design with a minimal mass

Minimize the mass Tie Tension Stiffness and length

prescribed,section free

E=r

Minimize the mass Beam Bending Stiffness,shape and

length ﬁxed,section free

E

1=2

=r

Minimize the mass Beam Bending Stiffness,width and

length ﬁxed,height free

E

1=3

=r

Minimize the mass Plate Bending Stiffness length width

ﬁxed,thickness free

E

1=3

=r

Minimize the mass Plate Com-

pression

Buckling load ﬁxed,

length width ﬁxed,

thickness free

E

1=3

=r

Minimize the mass Cylinder Internal

pressure

Imposed maximum

elastic strain,thickness

of the shell free

E=r

Strength design with a minimal mass

Minimize the mass Tie Traction Strength,length ﬁxed,

section free

s

e

=r

Minimize the mass Beam Bending Strength,length ﬁxed,

section free

s

e

2=3

=r

Minimize the mass Plate Bending Strength,length

and width ﬁxed,

thickness free

s

e

1=2

=r

Minimize the mass Cylinder Internal

pressure

Imposed pressure,the

materials shall not yield,

thickness of the shell free

s

e

=r

Brechet

20

Table 1.2.1 gives some standard performance indices currently used in

mechanical design.Many others have been derived,both for mechanical and

thermo-mechanical loading [1,4].

A simple way to use the performance index is with the so-called selection

maps shown in Figure 1.2.1:on a logarithmic scale the lines corresponding to

equal performances are straight lines whose slopes depend on the exponents

entering the performance index.Figure 1.2.1 shows one of these maps used

for stiff components at minimum mass.Materials for stiff ties should

maximize E=r,materials for stiff beams should maximize E

1/2

=r,and

materials for stiff plates should maximize E

1/3

=r.

These performance indices have a drawback,however:they are

concerned with time-independent design,the component is made so that it

FIGURE 1.2.1 Selection map for stiff light design [1].

1.2 Materials and Process Selection Methods

21

should fulﬁll its function when it starts being used,and it is assumed it

will be so for the rest of its life.Of course,this is rarely the case,and one

often has to design for a ﬁnite lifetime.As a consequence,for instance,in

designing for creep resistance or corrosion resistance,a new set of

performance indices involving rate equations (for creep or corrosion)

has been developed [8,9].The performance indices then depend not

only on the materials properties,but also on operating conditions such as

the load,or the dimensions,or the expected lifetime.For instance,large-scale

boilers are generally made out of steel,whereas small-scale boilers

are often made in copper.In principle,ﬁnite lifetime design is

possible within the framework of performance indices,but the data

available to effectively apply the method are much more difﬁcult to

gather systematically.

1.2.4 THE DESIGN PROCEDURE:SCREENING,

RANKING,AND FURTHER INFORMATION,

THE PROBLEM OF MULTIPLE

CRITERIA OPTIMIZATION

The previous method allows one to compare very different materials for a

given set of requirements formulated as a couple (constraint=objective).

However,in realistic situations,a set of requirements comprises many of these

‘‘elementary requirements.’’ Moreover,only part of the requirements can

indeed be formated that way.A typical selection procedure will proceed in

three steps:

1.At the screening stage,materials will be eliminated according to their

properties:only those that could possibly do the job will remain.For

instance,for a component in a turbine engine,the maximum operating

temperature should be around 800C:many materials won’t be able to

fulﬁll this basic requirement,and can be eliminated even without

looking for their other properties.

2.At the ranking stage,a systematic use of performance indices is made:

the problemis then,among admissible materials,to ﬁnd the ones which

will do the job most efﬁciently,that is,at the lowest cost,with the lowest

mass,or the smallest volume.The ranking will be made according to a

‘‘value function’’ which encompasses the various aspects of the set of

requirements.The problem of deﬁning such a value function for

multiple criteria optimization will be dealt with in the next paragraph.

Brechet

22

3.For the remaining candidates that are able to fulﬁll the set of

requirements efﬁciently,further information is often needed concerning

corrosion rates,wear rates,or possible surface treatments.These pieces

of information are scattered in the literature,and efﬁcient word-

searching methods are required to help with this step.At the same step,

the local conditions,or the availability of the different possible

materials,will also be a concern.

The three steps in the selection procedure are also a way to structure

process selection.The screening stage will rely on attributes such as the size of

the component and the materials fromwhich it is made.The ranking step will

need a rough comparative economic evaluation of the various processes,

involving the batch size and the production rate.The last step will depend on

the availability of the tooling and the will to invest.

It appears from these various aspects of the selection procedure that a key

issue is to build a ‘‘value function’’ that is able to provide one with a fair

comparison of the different possible solutions.The performance index

method is the ﬁrst step in building this value function.The second step is to

deal with the multicriteria nature of the selection process.This multicriteria

aspect can be conveniently classiﬁed in two categories:it might be a

multiconstraint problem,or a multiobjective problem (in any real situations,

it is both!).In a multiconstraint problem (such as designing a component

which should neither yield nor fail in fatigue),the problem is to identify the

limiting constraint.In order to do so,further knowledge on the load and the

dimensions is needed.A systematic method called ‘‘coupled equations’’ [10]

allows one to deal with this problem.In a multiobjective problem (such as

designing a component at minimumweight and minimumcost),one needs to

identify an ‘‘exchange coefﬁcient’’ [10] between the two objectives,for

instance,how much the user is ready to pay for saving weight.These

exchange coefﬁcients can be either obtained from a value analysis of the

product or from the analysis of existing solutions [4].They allow one to

compute a value function,which is the tool needed to rank the possible

solutions.Both the value analysis and the coupled equation method provide

one with an objective treatment of the multiple criteria optimization.

However,they require extra information compared to the simple performance

index method.When this information is not available,one needs to make use

of methods involving judgments.The most popular one is the ‘‘weight

coefﬁcients method,’’ which attributes to each criteria a percentage of

importance.The materials are then compared to an existing solution.It must

be stressed that the value function so constructed depends on the choice of

both the weighting factors and the reference material.Weighting factors are

difﬁcult to evaluate;moreover,multiple criteria often lead to no solution at all

1.2 Materials and Process Selection Methods

23

due to an excessive severity.Multiple optimization also implies the idea of

compromise between the various requirements.For this reason,algorithms

involving fuzzy logic methods [3] have been developed to deal with the

intrinsic fuzziness of the requirements (two values will be given,one above

which the satisfaction is complete,one under which the material will

be rejected).Proposed situations at the margin of full satisfaction will be

proposed for evaluation,and the value function will be constructed so that it

will give,for the same questions,the same evaluation as the user.This

technique bypasses the difﬁculty in giving a priori value coefﬁcients,since

they are then estimated from the evaluation-proposed solutions.However,

these methods still involve judgments (though in a controlled manner),and,

when possible,the objective methods should be preferred.

Once the value function is available,the selection problem becomes an

optimization one.When the database is ﬁnite,the optimization can be

performed by a simple screening of all the available solutions.The method has

been extended to the optimal design of multimaterials components such as

sandwich structures [11,12].The aim is then to simultaneously select the

skin,the core,and the geometry for a set of requirements involving stiffness

and strength,constraints on the thickness,objectives on the weight,or the

cost.For single criteria selection,an analytical method was derived [13].

For multiple criteria,such a method is no longer available,and the

selection requires one to compute the properties of a sandwich from

the properties of its components and its geometry,and to compare all the

possible choices.In order to ﬁnd the optimal solution,a genetic algorithmwas

used.The principle is to generate a population of sandwiches whose ‘‘genes’’

are the materials and the geometry.New sandwiches are generated,either by

mutation or by crossover between existing individuals,and the population is

kept constant in size by keeping the individuals alive with a

greater probability when their efﬁciency (measured by the value function)

is greater.In such a way,the algorithm converges very rapidly to a very

good solution.

1.2.5 MATERIALS SELECTION AND MATERIALS

DEVELOPMENT:THE ROLE OF MODELING

In the previous sections,we were interested in selecting materials and

processes to fulﬁl a set of requirements.The only modeling needed

at this stage is a simpliﬁed estimation of the mechanical behavior of the

component,together with a clear identiﬁcation of the constraints

and the objectives.The value function allowing one to estimate the efﬁciency

Brechet

24

of the different solutions is itself a simple linear combination of the

performance indices corresponding to the dominant constraints identiﬁed

by a predimensioning.

However,the same method has been applied to identify suitable materials

whose development would fulﬁll the requirements.Composite materials are

especially suitable for this exercise because their value relies partly on the

possibility of tayloring them for application [14,15].In order to design a

composite material,one has to identify the best choice for the matrix,for the

reinforcement,for the architecture of the reinforcement and its volume

fraction,and for the process to realize the component (which might be limited

by the shape to be realized).One needs relations,either empirical or based on

micromechanics models,between the properties of the components of the

composite and the properties of the material itself.Usually,the process itself

inﬂuences the properties obtained,which are lower than the properties of the

ideal composite that micromechanics models would provide.One could think

of introducing this feature in the modeling through interface properties,but it

is generally more convenient to store the information as ‘‘knock-down factors’’

on properties associated with a triplet matrix/reinforcement/process.

Another application of materials selection methods using mechanical

modeling is the optimal design of glass compositions for a given set of

requirements:since the properties are,within a certain range,linearly

related to the composition,optimization techniques such as a simplex

algorithmare well adapted to this problem.When a continuous variable,such

as the characteristics of a heat treatment for an alloy,is available and is

provided,either through metallurgical modeling or through empirical

correlation,the properties can be given as a function of this variable,

and materials selection methods are efﬁcient to design the best

treatment to be applied to ﬁt a set of requirements.However,the

explicit models available for relations between processes and properties

are relatively few.Recent developments using Neural net-works to

identify hidden correlation in databases of materials can also be

applied and coupled to selection methods in order to design the best

transformation processes.

Another recent development in selection methods aims at reverting the

problem,that is,ﬁnding potential applications for new materials [4,16,17].

Several strategies have been identiﬁed:for instance,one can explore a

database of applications (deﬁned by a set of requirements and existing

solutions) and ﬁnd the applications for which the new material is better than

the existing solutions.Another technique is to identify the performance

indices for which the new material seems better than usual materials,and

from there,to ﬁnd out the applications for which these performance indices

are relevant criteria.

1.2 Materials and Process Selection Methods

25

1.2.6 PROCESS SELECTION:STRUCTURING

THE EXPERTISE

In addition to selection by attributes of the process,which is efﬁcient in the

ﬁrst stages of selection,when one is confronted with a more speciﬁc problem,

such as selection of a deﬁnite cast aluminium alloy or a deﬁnite extruded

wrought alloy,or selection of a secondary process such as joining or surface

treatments,one is faced with the need to store expertise.For instance,for

selection of cast aluminium [3,18] alloys,the key issue is not to deﬁne the

performance index;the key issue is to select the alloy which will be possible

to cast without defects.Mold ﬁlling and hot tearing are the central concerns in

this problem.The ability to ﬁll a mold or to cast a component without cracks

depends on the alloy,on the geometry of the mold,and on the type of casting.

Ideally,one would wish to have models to deal with this question.In real life,

hot tearing criteria are not quantitatively reliable,mold-ﬁlling criteria are

totally empirical,and moreover,the properties of the cast alloy are dependent

on the solidiﬁcation conditions,that is,on the thickness of the component.

These dependences are part of what is known as expertise.The simplest way

to store this expertise is build the set of requirements according to a

predeﬁned questionnaire corresponding to the expert behavior.The second

option is to mimic the general tendency identiﬁed by the expert by a simple

mathematical function (for instance,capturing the tendency to increased hot

tearing with thinner parts of the component) and to tune the coefﬁcients of

these functions by comparing the results of selection by a software with the

results known fromthe case studies available to the expert.Along these lines,

selection methods for cast alloys [18],extruded alloys [19],joining methods

[20,21],and surface treatments [4,22] have been developed to capture

various expertises.Clearly,modeling is still needed to rationalize the

empirical rules commonly used (such as the shapes which can be extruded

or cast),or to evaluate the cost of a process (for instance,for joining by laser,

or for a surface treatment one needs to ﬁnd the best operating temperature,

power,speed,etc.).

1.2.7 CONCLUSIONS

The selection methods brieﬂy presented in this chapter are recent

developments.The use of modeling in these approaches is still in its infancy.

In the last ten years,general methods and software have been developed to

select materials,to select processes,and to deal with multidesign element

conception and with multicriteria set of requirements.

Brechet

26

TABLE 1.2.2 Selection softwares developed following the guidelines of the present paper.

Name of

the software Objectives of the software Comments=status

CMS Materials selection,graphical

selection using maps;many

databases,generic or specialized

Commercially available

CPS Process selection,graphical

method

Commercially available

CES Materials and process selection,

databases for materials,for

processes and links between

databases

Commercially available;

constructor facility for development

of dedicated databases

Fuzzymat Materials selection,multicriteria

and fuzzy logic-based selection

algorithm

Commercially available;

development of specialized

databases

CAMD Materials and process selection

for multidesign element

conceptions;expert system

to guide and analyze the

elaboration of requirements

Fuzzycast Selection of cast aluminium

alloys;databases:

alloys=processes=geometry

Property of Pechiney;expertise on

casting processes,design rules

Fuzzy-

composites

Design of polymer-based

composites;databases:resin,

reinforcements,processes,

and compatibilities

Sandwich

selector

Optimization of sandwich

structures;genetic algorithm

coupled with fuzzy logic

Fuzzyglass Optimization of glass

compositions;simplex coupled

with fuzzy logic

Property of SaintGobain

Astek Selection of joining methods;

databases:processes

and shapes

Property of CETIM

STS Selection of surface

treatments;database:

processes=materials=objectives

VCE Evaluation of exchange

coefﬁcients from

existing solutions

MAPS Investigation of possible

applications for a new material

1.2 Materials and Process Selection Methods

27

Table 1.2.2 gives a list of selection tools developed along the philosophy

described in this chapter.These generic methods have been specialized to

various classes of materials and processes.In special situations,a coupling

with modeling made possible the use of the present methods to develop new

materials or new structures (composites,sandwich structures).For speciﬁc

processes (casting,joining,extrusions,surface treatments),the selection

procedure developed was closer to an expert system,following a predeﬁned

questionnaire.Various methods of ﬁnding applications for a new material

have been put forward.Up to now,the choice has been to rely on empirical

knowledge when available,and to keep the selection procedure as transparent

and as objective as possible.The main reason for this paper to be included in a

book on models in mechanics is to express the need now to couple more

closely modeling to design so that one may go beyond empirical correlation

and optimize both the choice of materials and their future development.

REFERENCES

1.Ashby,M.(1999).Materials Selection in Mechanical Design,Butterworth Heinemann editor.

2.Esawi,A.(1994) PhD thesis,Cambridge University.

3.Bassetti,D.(1998) PhD thesis,Institut National Polytechnique de Grenoble.

4.Landru,D.(2000) PhD thesis,Institut National Polytechnique de Grenoble.

5.Granta Design,Cambridge Selection softwares:CMS (1995),CPS (1997),CES (1999).

6.Bassetti,Grenoble,Fuzzymat v3.0 (1997).

7.Landru,D.,and Brechet,Y.Grenoble,(1999).CAMD.

8.Ashby,M.,and Brechet,Y.Time Dependant Design (to be published).

9.Brechet,Y.,Ashby,M.,and Salvo,L.(2000).Methodes de choix des materiaux et des procedes,

Presses Universitaires de Lausanne.

10.Ashby,M.,(1997).ASTM-STP 1311,45,Computerization and Networking of Materials

Databases,Nishijima,S.,and Iwata,S.,eds.

11.Bassetti,D.,Brechet,Y.,Heiberg,G.,Lingorski,I.,Jantzen,A.,Pechambert,P.,and Salvo,L.

(1998).Materiaux et Techniques 5:31.

12.Deocon,J.,Salvo,L.,Lemoine,P.,Landru,D.,Brechet,Y.,and Leriche,R.(1999).Metal Foams

and Porous Metal Structures,Banhardt,J.,Ashby,M.,and Fleck,N.,eds.,MIT Verlag

Publishing,p.325.

13.Gibson,L.,and Ashby,M.(1999).Cellular solids,Cambridge University Press.

14.Pechambert,P.,Bassetti,D.,Brechet,Y.,and Salvo,L.(1996).ICCM7,London IOM,283.

15.Bassetti,D.,Brechet,Y.,Heiberg,G.,Lingorski,I.,Pechambert,P.,and Salvo,L.(1998).

Composite Design for Performance,p.88,Nicholson,P.,ed.,Lake Louise.

16.Landru,D.,Brechet,Y.(1996).Colloque Franco espagnol,p.41,Yavari,R.,ed.,Institut

National Polytechnique de Grenoble.

17.Landru,D.,Ashby,M.,and Brechet,Y.Finding New Applications for a Material (to be

published).

18.Lovatt,A.,Bassetti,D.,Shercliff,H.,and Brechet Y.(1999).Int.Journal Cast Metals Research

12:211.

19.Heiberg,G.,Brechet,Y.,Roven,H.,and Jensrud,O.Materials and Design (in press,2000).

Brechet

28

20.Lebacq,C.,Jeggy,T.,Brecht,Y.,and Salvo,L.(1998).Materiaux et Techniques 5:39.

21.Lebacq,C.,Brechet,Y.,Jeggy,T.,Salvo,L.,and Shercliff,H.(2000).Selection of joining

methods.Submitted to Materials and Design (see note 19).

22.Landru,D.,Esawi,A.,Brechet,Y.,and Ashby,M.(2000).Selection of surface treatments (to

be published).

1.2 Materials and Process Selection Methods

29

CHAP TE R

1.3

Size Effect on

Structural Strength

*

Z

DEN

$

EK

P.B

A

$

ZANT

Northwestern University,Evanston,Illinois

Contents

1.3.1 Introduction.................................32

1.3.2 History of Size Effect up to Weibull..........34

1.3.3 Power Scaling and the Case of No Size Effect.36

1.3.4 Weibull Statistical Size Effect................38

1.3.5 Quasi-Brittle Size Effect Bridging Plasticity

and LEFM,and its History...................40

1.3.6 Size Effect Mechanism:Stress Redistribution

and Energy Release..........................42

1.3.6.1 Scaling for Failure at Crack Initiation..43

1.3.6.2 Scaling for Failures with a Long Crack

or Notch.............................44

1.3.6.3 Size Effect on Postpeak Softening

and Ductility.........................47

1.3.6.4 Asymptotic Analysis of Size Effect

by Equivalent LEFM..................48

1.3.6.5 Size Effect Method for Measuring

Material Constants and R-Curve.......49

1.3.6.6 Critical Crack-tip Opening

Displacement,d

CTOD

..................50

1.3.7 Extensions,Ramiﬁcations,and Applications..50

1.3.7.1 Size Effects in Compression Fracture..50

*Thanks to the permission of Springer Verlag,Berlin,this article is reprinted from Archives of

Applied Mechanics (Ingenieur-Archiv) 69,703–725.A section on the reverse size effect in buckling

of sea ice and shells has been added,and some minor updates have been made.The ﬁgures

are the same.

Handbook of Materials Behavior Models

Copyright#2001 by Academic Press.All rights of reproduction in any form reserved.

30

1.3.7.2 Fracturing Truss Model for Concrete

and Boreholes in Rock...............51

1.3.7.3 Kink Bands in Fiber Composites.....52

1.3.7.4 Size Effects in Sea Ice...............52

1.3.7.5 Reverse Size Effect in Buckling of

Floating Ice or Cylindrical Shell......54

1.3.7.6 Inﬂuence of Crack Separation Rate,

Creep,and Viscosity.................55

1.3.7.7 Size Effect in Fatigue Crack Growth..56

1.3.7.8 Size Effect for Cohesive Crack Model

and Crack Band Model..............56

1.3.7.9 Size Effect via Nonlocal,Gradient,

or Discrete Element Models..........58

1.3.7.10 Nonlocal Statistical Generalization

of the Weibull Theory...............58

1.3.8 Other Size Effects...........................60

1.3.8.1 Hypothesis of Fractal Origin of

Size Effect..........................60

1.3.8.2 Boundary Layer,Singularity,

and Diffusion.......................61

1.3.9 Closing Remarks............................61

Acknowledgment..................................62

References and Bibliography.......................62

The article attempts a broad review of the problem of size effect or scaling of

failure,which has recently come to the forefront of attention because of its

importance for concrete and geotechnical engineering,geomechanics,and

arctic ice engineering,as well as in designing large load-bearing parts made of

advanced ceramics and composites,e.g.,for aircraft or ships.First the main

results of the Weibull statistical theory of random strength are brieﬂy

summarized and its applicability and limitations described.In this theory as

well as plasticity,elasticity with a strength limit,and linear elastic fracture

mechanics (LEFM),the size effect is a simple power law because no

characteristic size or length is present.Attention is then focused on the

deterministic size effect in quasi-brittle materials which,because of

the existence of a non-negligible material length characterizing the size

of the fracture process zone,represents the bridging between the simple

power-law size effects of plasticity and of LEFM.The energetic theory of

quasi-brittle size effect in the bridging region is explained,and then a host of

1.3 Size Effect on Structural Strength

31

recent reﬁnements,extensions,and ramiﬁcations are discussed.Comments on

other types of size effect,including that which might be associated with

the fractal geometry of fracture,are also made.The historical development

of the size effect theories is outlined,and the recent trends of research

are emphasized.

1.3.1 INTRODUCTION

The size effect is a problem of scaling,which is central to every physical

theory.In ﬂuid mechanics research,the problem of scaling continuously

played a prominent role for over a hundred years.In solid mechanics

research,though,the attention to scaling had many interruptions and became

intense only during the last decade.

Not surprisingly,the modern studies of nonclassical size effect,begun in

the 1970s,were stimulated by the problems of concrete structures,for which

there inevitably is a large gap between the scales of large structures (e.g.,

dams,reactor containments,bridges) and scales of laboratory tests.This gap

involves in such structures about one order of magnitude (even in the rare

cases when a full-scale test is carried out,it is impossible to acquire a

sufﬁcient statistical basis on the full scale).

The question of size effect recently became a crucial consideration in the

efforts to use advanced ﬁber composites and sandwiches for large ship hulls,

bulkheads,decks,stacks,and masts,as well as for large load-bearing fuselage

panels.The scaling problems are even greater in geotechnical engineering,

arctic engineering,and geomechanics.In analyzing the safety of an excavation

wall or a tunnel,the risk of a mountain slide,the risk of slip of a fault in the

earth crust,or the force exerted on an oil platform in the Arctic by a moving

mile-size ice ﬂoe,the scale jump from the laboratory spans many orders

of magnitude.

In most mechanical and aerospace engineering,on the other hand,the

problem of scaling has been less pressing because the structural components

can usually be tested at full size.It must be recognized,however,that even in

that case the scaling implied by the theory must be correct.Scaling is the most

fundamental characteristics of any physical theory.If the scaling properties of

a theory are incorrect,the theory itself is incorrect.

The size effect in solid mechanics is understood as the effect of the

characteristic structure size (dimension) D on the nominal strength s

N

of

structure when geometrically similar structures are compared.The nominal

stress (or strength,in case of maximum load) is deﬁned as s

N

¼ c

N

P=bD or

c

N

P=D

2

for two- or three-dimensional similarity,respectively;P¼ load

Ba$zant

32

(or load parameter),b structure thickness,and c

N

arbitrary coefﬁcient chosen

for convenience (normally c

N

¼ 1).So s

N

is not a real stress but a

load parameter having the dimension of stress.The deﬁnition of D can be

arbitrary (e.g.,the beam depth or half-depth,the beam span,the diagonal

dimension,etc.) because it does not matter for comparing geometrically

similar structures.

The basic scaling laws in physics are power laws in terms of D,for which

no characteristics size (or length) exists.The classical Weibull [113] theory of

statistical size effect caused by randomness of material strength is of this type.

During the 1970s it was found that a major deterministic size effect,

overwhelming the statistical size effect,can be caused by stress redistributions

caused by stable propagation of fracture or damage and the inherent

energy release.The law of the deterministic stable effect provides a way of

bridging two different power laws applicable in two adjacent size ranges.The

structure size at which this bridging transition occurs represents charac-

teristics size.

The material for which this new kind of size effect was identiﬁed ﬁrst,and

studied in the greatest depth and with the largest experimental effort by far,is

concrete.In general,a size effect that bridges the small-scale power law for

nonbrittle (plastic,ductile) behavior and the large-scale power law for brittle

behavior signals the presence of a certain non-negligible characteristics length

of the material.This length,which represents the quintessential property of

quasi-brittle materials,characterizes the typical size of material inhomogene-

ities or the fracture process zone (FPZ).Aside from concrete,other quasi-

brittle materials include rocks,cement mortars,ice (especially sea ice),

consolidated snow,tough ﬁber composites and particulate composites,

toughened ceramics,ﬁber-reinforced concretes,dental cements,bone and

cartilage,biological shells,stiff clays,cemented sands,grouted soils,coal,

paper,wood,wood particle board,various refractories and ﬁlled elastomers,

and some special tough metal alloys.Keen interest in the size effect

and scaling is now emerging for various ‘‘high-tech’’ applications of

these materials.

Quasi-brittle behavior can be attained by creating or enhancing material

inhomogeneities.Such behavior is desirable because it endows the structure

made from a material incapable of plastic yielding with a signiﬁcant energy

absorption capability.Long ago,civil engineers subconsciously but cleverly

engineered concrete structures to achieve and enhance quasi-brittle

characteristics.Most modern ‘‘high-tech’’ materials achieve quasi-brittle

characteristics in much the same way } by means of inclusions,embedded

reinforcement,and intentional microcracking (as in transformation toughen-

ing of ceramics,analogous to shrinkage microcracking of concrete).In effect,

they emulate concrete.

1.3 Size Effect on Structural Strength

33

In materials science,an inverse size effect spanning several orders of

magnitude must be tackled in passing fromnormal laboratory tests of material

strength to microelectronic components and micromechanisms.A material

that follows linear elastic fracture mechanics (LEFM) on the scale of

laboratory specimens of sizes from 1 to 10cm may exhibit quasi-brittle or

even ductile (plastic) failure on the scale of 0.1 to 100 microns.

The purpose of this article is to present a brief review of the basic results

and their history.For an in-depth review with several hundred literature

references,the recent article by Ba$zant and Chen [18] may be consulted.A

full exposition of most of the material reviewed here is found in the recent

book by Ba$zant and Planas [32],henceforth simply referenced as [BP].The

problem of scale bridging in the micromechanics of materials,e.g.,the

relation of dislocation theory of continuum plasticity,is beyond the scope of

this review (it is treated in this volume by Hutchinson).

1.3.2 HISTORY OF SIZE EFFECT

UP TO WEIBULL

Speculations about the size effect can be traced back to Leonardo da Vinci

(1500s) [118].He observed that ‘‘among cords of equal thickness the

longest is the least strong,’’ and proposed that ‘‘a cord is so much stronger as it

is shorter,’’ implying inverse proportionality.A century later,Galileo Galilei

[64] the inventor of the concept of stress,argued that Leonardo’s size effect

cannot be true.He further discussed the effect of the size of an animal

on the shape of its bones,remarking that bulkiness of bones is the weakness of

the giants.

A major idea was spawned by Mariotte [82].Based on his extensive

experiments,he observed that ‘‘a long rope and a short one always support the

same weight unless that in a long rope there may happen to be some faulty

place in which it will break sooner than in a shorter,’’ and proposed the

principle of ‘‘the inequality of matter whose absolute resistance is less in one

place than another.’’ In other words,the larger the structure,the greater is the

probability of encountering in it an element of low strength.This is the basic

idea of the statistical theory of size effect.

Despite no lack of attention,not much progress was achieved for two and

half centuries,until the remarkable work of Grifﬁth [66] the founder of

fracture mechanics.He showed experimentally that the nominal strength of

glass ﬁbers was raised from 42,300 psi to 491,000 psi when the diameter

decreased from0.0042 in.to 0.00013 in.,and concluded that ‘‘the weakness of

isotropic solids...is due to the presence of discontinuities or ﬂaws....The

Ba$zant

34

effective strength of technical materials could be increased 10 or 20 times at

least if these ﬂaws could be eliminated.’’ In Grifﬁth’s view,however,the ﬂaws

or cracks at the moment of failure were still only microscopic;their random

distribution controlled the macroscopic strength of the material but did not

invalidate the concept of strength.Thus,Grifﬁth discovered the physical basis

of Mariotte’s statistical idea but not a new kind of size effect.

The statistical theory of size effect began to emerge after Peirce [92]

formulated the weakest-link model for a chain and introduced the extreme

value statistics which was originated by Tippett [107] and Fr

!

echet [57] and

completely described by Fischer and Tippett [58],who derived the Weibull

distribution and proved that it represents the distribution of the minimum of

any set of very many randomvariables that have a threshold and approach the

threshold asymptotically as a power function of any positive exponent.

Reﬁnements were made by von Mises [108] and others (see also

[62,63,103,56].The capstone of the statistical theory of strength was laid

by Weibull [113] (also [114–116]).On a heuristic and experimental basis,he

concluded that the tail distribution of low strength values with an extremely

small probability could not be adequately represented by any of the previously

known distributions and assumed the cumulative probability distribution of

the strength of a small material element to be a power function of the strength

difference form a ﬁnite or zero threshold.The resulting distribution of

minimum strength,which was the same as that derived by Fischer and Tippet

[58] in a completely different context,came to be known as the Weibull

distribution.Others [62,103] later offered a theoretical justiﬁcation by means

of a statistical distribution of microscopic ﬂaws or microcracks.Reﬁnements

and applications to metals and ceramics (fatigue embrittlement,cleavage

toughness of steels at a low and brittle-ductile transition temperatures,

evaluation of scatter of fracture toughness data) have continued until today

[37,56,77,101].Applications of Weibull’s theory to fatigue embrittled metals

and to ceramics have been researched thoroughly [75,76].Applications to

concrete,where the size effect has been of the greatest concern,have been

studied by Zaitsev and Wittmann [122],Mihashi and Izumi [88],Wittmann

and Zaitsev [121],Zech and Wittmann [123],Mihashi [84],Mihashi and

Izumi [85] Carpinteri [41,42],and others.

Until about 1985,most mechanicians paid almost no attention to the

possibility of a deterministic size effect.Whenever a size effect was detected in

tests,it was automatically assumed to be statistical,and thus its study was

supposed to belong to statisticians rather than mechanicians.The reason

probably was that no size effect is exhibited by the classical continuum

mechanics in which the failure criterion is written in terms of stresses and

strains (elasticity with strength limit,plasticity and viscoplasticity,as well

as fracture mechanics of bodies containing only microscopic cracks or

1.3 Size Effect on Structural Strength

35

ﬂaws) [8].The subject was not even mentioned by S.P.Timoshenko in 1953

in his monumental History of the Strength of Materials.

The attitude,however,changed drastically in the 1980s.In consequence of the

well-funded research in concrete structures for nuclear power plants,theories

exhibiting a deterministic size effect have developed.We will discuss it later.

1.3.3 POWER SCALING AND THE CASE OF

NO SIZE EFFECT

It is proper to explain ﬁrst the simple scaling applicable to all physical systems

that involve no characteristic length.Let us consider geometrically similar

systems,for example,the beams shown in Figure 1.3.1a,and seek to deduce

the response Y (e.g.,the maximum stress or the maximum deﬂection) as a

function of the characteristic size (dimension) D of the structure;Y ¼ Y

0

f ðDÞ

FIGURE 1.3.1 a.Top left:Geometrically similar structures of different sizes.b.Top right:Power

scaling laws.c.Bottom.Size effect lawfor quasi-brittle failures bridging the power law of plasticity

(horizontal asymptote) and the power law of LEFM (inclined asymptote).

Ba$zant

36

where u is the chosen unit of measurement (e.g.,1m,1mm).We imagine

three structure sizes 1,D,and D

0

(Figure 1.3.1a).If we take size 1 as the

reference size,the responses for sizes D and D

0

are Y ¼ f ðDÞ and Y

0

¼ f ðD

0

Þ.

However,since there is no characteristic length,we can also take size D as the

reference size.Consequently,the equation

f ðD

0

Þ=f ðDÞ ¼ f ðD

0

=DÞ ð1Þ

must hold ([8,18];for ﬂuid mechanics [2,102]).This is a functional equation

for the unknown scaling law f ðDÞ.It has one and only one solution,namely,

the power law:

f ðDÞ ¼ ðD=c

1

Þ

s

ð2Þ

where s ¼ constant and c

1

is a constant which is always implied as a unit of

length measurement (e.g.,1m,1mm).Note that c

1

cancels out of Eq.2 when

the power function (Eq.1) is substituted.

On the other hand,when,for instance,f ðDÞ ¼ logðD=c

1

Þ,Eq.1 is not

satisﬁed and the unit of measurement,c

1

,does not cancel out.So,the

logarithmic scaling could be possible only if the system possessed a

characteristic length related to c

1

.

The power scaling must apply for every physical theory in which there is

no characteristic length.In solid mechanics such failure theories include

elasticity with a strength limit,elastoplasticity,and viscoplasticity,as well as

LEFM (for which the FPZ is assumed shrunken into a point).

To determine exponent s,the failure criterion of the material must be taken

into account.For elasticity with a strength limit (strength theory),or

plasticity (or elastoplasticity) with a yield surface expressed in terms of

stresses or strains,or both,one ﬁnds that s ¼ 0 when response Y represents

the stress or strain (for example,the maximum stress,or the stress at certain

homologous points,or the nominal stress at failure) [8].Thus,if there is no

characteristic dimension,all geometrically similar structures of different sizes

must fail at the same nominal stress.By convention,this came to be known as

the case of no size effect.

In LEFM,on the other hand,s ¼ 1=2,provided that the geometrically

similar structures with geometrically similar cracks or notches are considered.

This may be generally demonstrated with the help of Rice’s J-integral [8].

If log s

N

is plotted versus log D,the power law is a straight line (Figure

1.3.1b).For plasticity,or elasticity with a strength limit,the exponent of the

power law vanishes,i.e.,the slope of this line is 0,while for LEFMthe slope is

1/2 [8].An emerging ‘‘hot’’ subject is the quasi-brittle materials and

structures,for which the size effect bridges these two power laws.

It is interesting to note that critical stress for elastic buckling of beams,

frames,and plates exhibits also no size effect,i.e.,is the same for

1.3 Size Effect on Structural Strength

37

geometrically similar structures of different sizes.However,this is not true for

beams on elastic foundation and for shells [16].

1.3.4 WEIBULL STATISTICAL SIZE EFFECT

The classical theory of size effect has been statistical.Three-dimensional

continuous generalization of the weakest link model for the failure of a chain

of links of random strength (Fig.1.3.2a) leads to the distribution

P

f

ðs

N

Þ ¼ 1 exp

Z

V

c½rðvÞ;s

N

ÞdVðvÞ

s

which represents the probability that a structure that fails as soon as

macroscopic fracture initiates from a microcrack (or a some ﬂaw) somewhere

in the structure;s ¼ stress tensor ﬁeld just before failure,v ¼ coordinate

vector,V ¼ volume of structure,and cðrÞ ¼function giving the spatial

concentration of failure probability of material (¼ V

1

r

failure probability of

material representative volume V

r

) [62];cðrÞ

P

i

P

1

ðs

i

Þ=V

0

where

s

i

¼ principal stresses (i ¼ 1;2;3) and P

1

ðsÞ¼ failure probability (cumula-

tive) of the smallest possible test specimen of volume V

0

(or representative

FIGURE 1.3.2 a.Left:Chain with many links of random strength.b.Right top:Failure

probability of a small element.c.Right bottom:Structures with many microcracks of different

probabilities to become critical.

Ba$zant

38

volume of the material) subject to uniaxial tensile stress s;

P

1

ðsÞ ¼

s s

u

s

0

m

ð4Þ

[113] where m,s

0

,s

1

¼ material constants (m ¼ Weibull modulus,usually

between 5 and 50;s

0

¼ scale parameter;s

u

¼ strength threshold,which may

usually be taken as 0) and V

0

¼ reference volume understood as the volume

of specimens on which cðsÞ was measured.For specimens under uniform

uniaxial stress (and s

u

¼ 0),Eqs.3 and 4 lead to the following simple

expressions for the mean and coefﬁcient of variation of the nominal strength:

%

s

N

¼ s

0

Gð1 þm

1

ÞðV

0

=VÞ

1=m

o ¼ ½Gð1 þ2m

1

Þ=G

2

ð1 þm

1

Þ 1

1=2

ð5Þ

where G is the gamma function.Since o depends only on m,it is often used

for determining m form the observed statistical scatter of strength of identical

test specimens.The expression for

%

s

N

includes the effect of volume V which

depends on size D.In general,for structures with nonuniform multi-

dimensional stress,the size effect of Weibull theory (for s

r

0) is

of the type

%

s

N

/D

n

d

=m

ð6Þ

where n

d

¼ 1,2,or 3 for uni-,two- or three-dimensional similarity.

In view of Eq.5,the value s

W

¼ s

N

ðV=V

0

Þ

1=m

for a uniformity stressed

specimen can be adopted as a size-independent stress measure called the

Weibull stress.Taking this viewpoint,Beremin [37] proposed taking into

account the nonuniform stress in a large crack-tip plastic zone by the so-

called Weibull stress:

s

W

¼

X

i

s

I

m

i

V

i

V

0

!

1=m

ð7Þ

where V

i

ði ¼ 1;2;...N

W

Þ are elements of the plastic zone having maximum

principal stress s

Ii

.Ruggieri and Dodds [101] replaced the sumin Eq.5 by an

integral;see also Lei et al.[77].Equation 7,however,considers only the

crack-tip plastic zone whose size which is almost independent of D.

Consequently,Eq.7 is applicable only if the crack at the moment of failure

is not yet macroscopic,still being negligible compared to structural dimensions.

As far as quasi-brittle structures are concerned,applications of the classic

Weibull theory face a number of serious objections:

1.The fact that in Eq.6 the size effect is a power law implies the absence of

any characteristic length.But this cannot be true if the material contains

sizable inhomogeneities.

1.3 Size Effect on Structural Strength

39

2.The energy release due to stress redistributions caused by macroscopic

FPZ or stable crack growth before P

max

gives rise to a deterministic size

effect which is ignored.Thus the Weibull theory is valid only if the

structure fails as soon as a microscopic crack becomes macroscopic.

3.Every structure is mathematically equivalent to a uniaxially stressed bar

(or chain,Fig.1.3.2),which means that no information on the

structural geometry and failure mechanism is taken into account.

4.The size effect differences between two- and three-dimensional

similarity (n

d

¼2 or 3) are predicted much too large.

5.Many tests of quasi-brittle materials (e.g.,diagonal shear failure of

reinforced concrete beams) show a much stronger size effect than

predicted by the Weibull theory ([BP]),and the review in Ba$zant [9]).

6.The classical theory neglects the spatial correlations of material failure

probabilities of neighboring elements caused by nonlocal properties of

damage evolution (while generalizations based on some phenomen-

ological load-sharing hypotheses have been divorced from mechanics).

7.When Eq.5 is ﬁtted to the test data on statistical scatter for specimens of

one size (V ¼ const.) and when Eq.6 is ﬁtted to the mean test data on

the effect of size or V (of unnotched plain concrete specimens),the

optimum values of Weibull exponent m are very different,namely,

m ¼ 12 and m ¼ 24,respectively.If the theory were applicable,these

values would have to coincide.

In view of these limitations,among concrete structures Weibull theory

appears applicable to some extremely thick plain (unreinforced) structures,

e.g.,the ﬂexure of an arch dam acting as a horizontal beam (but not for

vertical bending of arch dams or gravity dams because large vertical

compressive stresses cause long cracks to grow stably before the maximum

load).Most other plain concrete structures are not thick enough to prevent

the deterministic size effect from dominating.Steel or ﬁber reinforcement

prevents it as well.

1.3.5 QUASI-BRITTLE SIZE EFFECT BRIDGING

PLASTICITY AND LEFM,AND ITS HISTORY

Qausi-brittle materials are those that obey on a small scale the theory of

plasticity (or strength theory),characterized by material strength or yield

limit s

0

,and on a large scale the LEFM,characterized by fracture energy G

f

.

While plasticity alone,as well as LEFM alone,possesses no characteristics

length,the combination of both,which must be considered for the bridging of

plasticity and LEFM,does.Combination of s

0

and G

f

yields Irwin’s (1958)

Ba$zant

40

characteristic length (material length):

‘

0

¼

EG

f

s

2

0

ð8Þ

which approximately characterizes the size of the FPZ (E ¼ Young

0

s elastic

modulus).So the key to the deterministic quasi-brittle size effect is a

combination of the concept of strength or yield with fracture mechanics.

In dynamics,this further implies the existence of a characteristic time

(material time):

t

0

¼ ‘

0

=v ð9Þ

representing the time a wave of velocity v takes to propagate the distance ‘

0

.

After LEFMwas ﬁrst applied to concrete [72],it was found to disagree with

test results [74,78,111,112].Leicester [78] tested geometrically similar

notched beams of different sizes,ﬁtted the results by a power law,s

N

/D

2n

,

and observed that the optimum n was less than 1/2,the value required by

LEFM.The power law with a reduced exponent of course ﬁts the test data in

the central part of the transitional size range well but does not provide the

bridging of the ductile and LEFMsize effects.An attempt was made to explain

the reduced exponent value by notches of a ﬁnite angle,which,however,is

objectionable for two reasons:(i) notches of a ﬁnite angle cannot propagate

(rather,a crack must emanate from the notch tip),and (ii) the singular stress

ﬁeld of ﬁnite-angle notches gives a zero ﬂux of energy into the notch tip.Like

Weibull theory,Leicester’s power law also implied the nonexistence of a

characteristic length (see Ba$zant and Chen [18],Eqs.1–3),which cannot be

the case for concrete because of the large size of its inhomogeneities.More

extensive tests of notched geometrically similar concrete beams of different

sizes were carried out by Walsh [111,112].Although he did not attempt a

mathematical formulation,he was ﬁrst to make the doubly logarithmic plot of

nominal strength versus size and observe that it is was transitional between

plasticity and LEFM.

An important advance was made by Hillerborg et al.[68] (also Peterson

[93]).Inspired by the softening and plastic FPZ models of Barenblatt [2,3]

and Dugdale [55],they formulated the cohesive (or ﬁctitious) crack model

characterized by a softening stress-displacement law for the crack opening

and showed by ﬁnite element calculations that the failures of unnotched plain

concrete beams in bending exhibit a deterministic size effect,in agreement

with tests of the modulus of rupture.

Analyzing distributed (smeared) cracking damage,Ba$zant [4] demon-

strated that its localization into a crack band engenders a deterministic size

effect on the postpeak deﬂections and energy dissipation of structures.The

effect of the crack band is approximately equivalent to that of a long fracture

1.3 Size Effect on Structural Strength

41

with a sizable FPZ at the tip.Subsequently,using an approximate energy

release analysis,Ba$zant [5] derived for the quasi-brittle size effect in

structures failing after large stable crack growth the following approximate

## Σχόλια 0

Συνδεθείτε για να κοινοποιήσετε σχόλιο